# Electronic Supplementary Material (ESI) for Chemical Communications.
# This journal is © The Royal Society of Chemistry 2020

####################################################################### 
# 
# This file contains crystal structure data downloaded from the 
# Cambridge Structural Database (CSD) hosted by the Cambridge 
# Crystallographic Data Centre (CCDC).
# 
# Full information about CCDC data access policies and citation 
# guidelines are available at http://www.ccdc.cam.ac.uk/access/V1 
# 
# Audit and citation data items may have been added by the CCDC. 
# Please retain this information to preserve the provenance of 
# this file and to allow appropriate attribution of the data. 
# 
#######################################################################

data_190124-2_sq
_database_code_depnum_ccdc_archive 'CCDC 1964911'
loop_
_audit_author_name
_audit_author_address
'Ming Xu'
;Northeast Normal University
China
;
_audit_update_record             
;
2019-11-09 deposited with the CCDC.	2019-12-19 downloaded from the CCDC.
;
_audit_creation_date             2019-05-06
_audit_creation_method           
;
Olex2 1.2
(compiled 2018.05.29 svn.r3508 for OlexSys, GUI svn.r5506)
;
_shelx_SHELXL_version_number     2014/7
_chemical_name_common            ?
_chemical_name_systematic        ?
_chemical_formula_moiety         'K6 Mo18 O78 P2 Ti2, 10(O)'
_chemical_formula_sum            'K6 Mo18 O88 P2 Ti2'
_chemical_formula_weight         3527.26
_chemical_melting_point          ?
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
K K 0.2009 0.2494 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Mo Mo -1.6832 0.6857 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
P P 0.1023 0.0942 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ti Ti 0.2776 0.4457 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'

_shelx_space_group_comment       
;
The symmetry employed for this shelxl refinement is uniquely defined
by the following loop, which should always be used as a source of
symmetry information in preference to the above space-group names.
They are only intended as comments.
;
_space_group_crystal_system      triclinic
_space_group_IT_number           2
_space_group_name_H-M_alt        'P -1'
_space_group_name_Hall           '-P 1'
loop_
_space_group_symop_operation_xyz
'x, y, z'
'-x, -y, -z'

_cell_length_a                   12.3750(4)
_cell_length_b                   13.5901(5)
_cell_length_c                   16.7251(7)
_cell_angle_alpha                103.174(3)
_cell_angle_beta                 110.846(3)
_cell_angle_gamma                94.834(3)
_cell_volume                     2516.86(17)
_cell_formula_units_Z            1
_cell_measurement_reflns_used    9864
_cell_measurement_temperature    273
_cell_measurement_theta_max      25.124
_cell_measurement_theta_min      2.583
_shelx_estimated_absorpt_T_max   0.688
_shelx_estimated_absorpt_T_min   0.577
_exptl_absorpt_coefficient_mu    2.690
_exptl_absorpt_correction_T_max  0.68
_exptl_absorpt_correction_T_min  0.53
_exptl_absorpt_correction_type   ?
_exptl_absorpt_process_details   ad
_exptl_absorpt_special_details   ?
_exptl_crystal_colour            'clear light colourless'
_exptl_crystal_colour_lustre     clear
_exptl_crystal_colour_modifier   light
_exptl_crystal_colour_primary    colourless
_exptl_crystal_density_diffrn    2.327
_exptl_crystal_density_meas      ?
_exptl_crystal_density_method    ?
_exptl_crystal_description       block
_exptl_crystal_F_000             1648
_exptl_crystal_size_max          0.23
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.15
_exptl_transmission_factor_max   ?
_exptl_transmission_factor_min   ?
_diffrn_reflns_av_R_equivalents  0.0310
_diffrn_reflns_av_unetI/netI     0.0607
_diffrn_reflns_Laue_measured_fraction_full 0.991
_diffrn_reflns_Laue_measured_fraction_max 0.829
_diffrn_reflns_limit_h_max       16
_diffrn_reflns_limit_h_min       -16
_diffrn_reflns_limit_k_max       18
_diffrn_reflns_limit_k_min       -16
_diffrn_reflns_limit_l_max       19
_diffrn_reflns_limit_l_min       -22
_diffrn_reflns_number            19103
_diffrn_reflns_point_group_measured_fraction_full 0.991
_diffrn_reflns_point_group_measured_fraction_max 0.829
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         29.373
_diffrn_reflns_theta_min         3.488
_diffrn_ambient_temperature      273.0
_diffrn_detector_area_resol_mean ?
_diffrn_measured_fraction_theta_full 0.991
_diffrn_measured_fraction_theta_max 0.829
_diffrn_measurement_device_type  'multiwire proportional'
_diffrn_measurement_method       'phi and omega scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_source                   ?
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                8762
_reflns_number_total             11489
_reflns_special_details          
;
 Reflections were merged by SHELXL according to the crystal
 class for the calculation of statistics and refinement.
 
 Structure factors included contributions from the .fab file.
 
 _reflns_Friedel_fraction is defined as the number of unique
 Friedel pairs measured divided by the number that would be
 possible theoretically, ignoring centric projections and
 systematic absences.
;
_reflns_threshold_expression     'I > 2σ(I)'
_computing_cell_refinement       ?
_computing_data_collection       ?
_computing_data_reduction        ?
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_computing_structure_solution    'olex2.solve (Bourhis et al., 2015)'
_refine_diff_density_max         2.753
_refine_diff_density_min         -1.313
_refine_diff_density_rms         0.193
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.040
_refine_ls_hydrogen_treatment    undef
_refine_ls_matrix_type           full
_refine_ls_number_parameters     513
_refine_ls_number_reflns         11489
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.0688
_refine_ls_R_factor_gt           0.0515
_refine_ls_restrained_S_all      1.040
_refine_ls_shift/su_max          0.001
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details     
'w=1/[σ²(Fo²)+(0.0755P)²+9.0024P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.1452
_refine_ls_wR_factor_ref         0.1618
_refine_special_details          ?
_olex2_refinement_description    
;
;
_atom_sites_solution_hydrogens   .
_atom_sites_solution_primary     iterative
_atom_sites_solution_secondary   ?
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_site_symmetry_order
_atom_site_calc_flag
_atom_site_refinement_flags_posn
_atom_site_refinement_flags_adp
_atom_site_refinement_flags_occupancy
_atom_site_disorder_assembly
_atom_site_disorder_group
Mo1 Mo 0.57560(5) 0.46427(5) 0.23763(5) 0.03431(17) Uani 1 1 d . . . . .
Mo2 Mo 0.57494(6) 0.23956(6) 0.28790(5) 0.03737(17) Uani 1 1 d . . . . .
Mo3 Mo 0.32759(6) 0.12737(5) 0.33660(4) 0.03616(17) Uani 1 1 d . . . . .
Mo4 Mo 0.10897(6) 0.25581(6) 0.33677(4) 0.03550(17) Uani 1 1 d . . . . .
Mo5 Mo 0.09836(6) 0.49920(5) 0.26984(4) 0.03233(16) Uani 1 1 d . . . . .
Mo6 Mo 0.32351(5) 0.60056(5) 0.21911(5) 0.03236(16) Uani 1 1 d . . . . .
Mo7 Mo 0.28184(5) 0.34456(5) 0.03908(4) 0.02704(15) Uani 1 1 d . . . . .
Mo8 Mo 0.27930(5) 0.12221(5) 0.10000(4) 0.02870(15) Uani 1 1 d . . . . .
Mo9 Mo 0.04186(5) 0.23862(5) 0.09081(4) 0.02595(14) Uani 1 1 d . . . . .
Ti1 Ti 0.08626(11) 0.45651(10) 0.06938(9) 0.0291(3) Uani 1 1 d . . . . .
K1 K 0.6745(3) 0.4998(2) 0.51072(19) 0.0904(9) Uani 1 1 d . . . . .
K2 K -0.2436(2) 0.12610(16) -0.15028(16) 0.0734(8) Uani 1 1 d . . . . .
K3 K 0.2002(3) -0.1073(3) -0.1446(2) 0.0952(10) Uani 1 1 d . . . . .
P1 P 0.32197(14) 0.35375(13) 0.26235(11) 0.0231(3) Uani 1 1 d . . . . .
O1 O 0.6185(4) 0.3317(4) 0.2272(4) 0.0418(13) Uani 1 1 d . . . . .
O2 O 0.4322(4) 0.3831(4) 0.1067(3) 0.0310(11) Uani 1 1 d . . . . .
O3 O 0.4653(4) 0.5570(4) 0.2321(4) 0.0358(12) Uani 1 1 d . . . . .
O4 O 0.6637(5) 0.5192(5) 0.3477(4) 0.0510(16) Uani 1 1 d . . . . .
O5 O 0.6519(5) 0.5105(5) 0.1833(4) 0.0485(15) Uani 1 1 d . . . . .
O6 O 0.4542(4) 0.3656(4) 0.2839(3) 0.0305(11) Uani 1 1 d . . . . .
O7 O 0.4643(4) 0.1656(4) 0.3161(4) 0.0406(13) Uani 1 1 d . . . . .
O8 O 0.4318(4) 0.1718(4) 0.1545(3) 0.0351(12) Uani 1 1 d . . . . .
O9 O 0.6627(5) 0.3104(5) 0.3945(4) 0.0528(16) Uani 1 1 d . . . . .
O10 O 0.6549(5) 0.1486(5) 0.2643(4) 0.0544(16) Uani 1 1 d . . . . .
O11 O 0.1658(5) 0.1299(4) 0.3196(4) 0.0417(13) Uani 1 1 d . . . . .
O12 O 0.2561(4) 0.0930(4) 0.1910(3) 0.0319(11) Uani 1 1 d . . . . .
O13 O 0.3876(6) 0.1829(5) 0.4496(4) 0.0559(17) Uani 1 1 d . . . . .
O14 O 0.3241(5) -0.0014(5) 0.3273(4) 0.0486(15) Uani 1 1 d . . . . .
O15 O 0.2900(4) 0.2936(4) 0.3200(3) 0.0326(11) Uani 1 1 d . . . . .
O16 O 0.0882(5) 0.3874(4) 0.3152(4) 0.0402(13) Uani 1 1 d . . . . .
O17 O 0.0480(4) 0.2115(4) 0.1901(3) 0.0313(11) Uani 1 1 d . . . . .
O18 O 0.1868(6) 0.3045(5) 0.4490(4) 0.0499(15) Uani 1 1 d . . . . .
O19 O -0.0278(5) 0.2084(5) 0.3287(4) 0.0507(16) Uani 1 1 d . . . . .
O20 O 0.1471(4) 0.5695(4) 0.1891(3) 0.0331(11) Uani 1 1 d . . . . .
O21 O 0.0519(4) 0.3856(4) 0.1471(3) 0.0261(10) Uani 1 1 d . . . . .
O22 O 0.1785(5) 0.5922(5) 0.3669(4) 0.0471(14) Uani 1 1 d . . . . .
O23 O -0.0394(5) 0.5272(5) 0.2420(4) 0.0480(15) Uani 1 1 d . . . . .
O24 O 0.2861(4) 0.4593(4) 0.2787(3) 0.0298(11) Uani 1 1 d . . . . .
O26 O 0.3597(5) 0.6760(5) 0.3241(4) 0.0517(16) Uani 1 1 d . . . . .
O27 O 0.3207(5) 0.6871(5) 0.1602(4) 0.0484(15) Uani 1 1 d . . . . .
O28 O 0.2704(4) 0.2055(4) 0.0092(3) 0.0337(11) Uani 1 1 d . . . . .
O29 O 0.0982(4) 0.3203(4) 0.0124(3) 0.0294(11) Uani 1 1 d . . . . .
O30 O 0.2540(4) 0.4752(4) 0.1031(3) 0.0259(10) Uani 1 1 d . . . . .
O31 O 0.2691(5) 0.3710(4) -0.0579(4) 0.0404(13) Uani 1 1 d . . . . .
O32 O 0.2548(4) 0.2911(3) 0.1618(3) 0.0245(10) Uani 1 1 d . . . . .
O33 O 0.1006(4) 0.1299(4) 0.0462(3) 0.0297(11) Uani 1 1 d . . . . .
O34 O 0.2692(5) 0.0050(4) 0.0312(4) 0.0412(13) Uani 1 1 d . . . . .
O35 O -0.1038(4) 0.2070(4) 0.0224(4) 0.0380(12) Uani 1 1 d . . . . .
O36 O -0.0087(7) 0.0276(6) -0.1377(5) 0.073(2) Uani 1 1 d . . . . .
O37 O 0.1873(7) -0.3109(7) -0.1898(7) 0.088(3) Uani 1 1 d . . . . .
O39 O 0.5066(8) 0.6106(7) 0.4691(6) 0.096(3) Uiso 1 1 d . . . . .
O45 O -0.0778(4) 0.4666(5) 0.0166(4) 0.0476(15) Uani 1 1 d . . . . .
O38 O 0.3401(13) 0.2532(9) 0.6141(8) 0.146(5) Uani 1 1 d . . . . .
O40 O -0.1076(11) 0.6392(11) 0.3964(9) 0.148(5) Uiso 1 1 d . . . . .
O41 O -0.1609(5) 0.6885(4) 0.2427(3) 0.0413(13) Uani 1 1 d . . . . .
O42 O 0.0526(9) 0.7479(7) 0.1697(5) 0.092(3) Uani 1 1 d . . . . .
O43 O -0.2458(5) 0.4046(5) 0.0585(4) 0.0450(14) Uani 1 1 d . . . . .
O44 O -0.0480(11) 0.0704(8) -0.2965(7) 0.120(4) Uani 1 1 d . . . . .


_geom_special_details            
;
 All esds (except the esd in the dihedral angle between two l.s. planes)
 are estimated using the full covariance matrix.  The cell esds are taken
 into account individually in the estimation of esds in distances, angles
 and torsion angles; correlations between esds in cell parameters are only
 used when they are defined by crystal symmetry.  An approximate (isotropic)
 treatment of cell esds is used for estimating esds involving l.s. planes.
;
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
_geom_bond_publ_flag
Mo1 O1 1.909(6) . ?
Mo1 O2 2.228(5) . ?
Mo1 O3 1.927(5) . ?
Mo1 O4 1.715(6) . ?
Mo1 O5 1.698(5) . ?
Mo1 O6 2.370(5) . ?
Mo2 O1 1.935(6) . ?
Mo2 O6 2.363(5) . ?
Mo2 O7 1.884(5) . ?
Mo2 O8 2.223(5) . ?
Mo2 O9 1.717(6) . ?
Mo2 O10 1.710(6) . ?
Mo3 K2 3.854(2) 2 ?
Mo3 O7 1.896(5) . ?
Mo3 O11 1.925(6) . ?
Mo3 O12 2.194(5) . ?
Mo3 O13 1.717(6) . ?
Mo3 O14 1.717(6) . ?
Mo3 O15 2.401(5) . ?
Mo4 K1 3.807(3) 2_666 ?
Mo4 K3 4.004(3) 2 ?
Mo4 O11 1.904(6) . ?
Mo4 O15 2.384(5) . ?
Mo4 O16 1.924(6) . ?
Mo4 O17 2.210(5) . ?
Mo4 O18 1.712(6) . ?
Mo4 O19 1.707(6) . ?
Mo5 Ti1 3.2158(14) . ?
Mo5 K1 3.742(3) 2_666 ?
Mo5 O16 1.860(5) . ?
Mo5 O20 2.042(5) . ?
Mo5 O21 2.120(5) . ?
Mo5 O22 1.711(6) . ?
Mo5 O23 1.701(6) . ?
Mo5 O24 2.391(5) . ?
Mo6 Ti1 3.2075(14) . ?
Mo6 O3 1.854(5) . ?
Mo6 O20 2.041(5) . ?
Mo6 O24 2.437(5) . ?
Mo6 O26 1.697(6) . ?
Mo6 O27 1.693(6) . ?
Mo6 O30 2.113(5) . ?
Mo7 Ti1 3.0937(15) . ?
Mo7 O2 1.756(5) . ?
Mo7 O28 1.821(5) . ?
Mo7 O29 2.135(5) . ?
Mo7 O30 1.979(5) . ?
Mo7 O31 1.696(5) . ?
Mo7 O32 2.445(5) . ?
Mo8 K2 3.687(2) 2 ?
Mo8 O8 1.768(5) . ?
Mo8 O12 1.767(5) . ?
Mo8 O28 2.069(5) . ?
Mo8 O32 2.385(5) . ?
Mo8 O33 2.092(5) . ?
Mo8 O34 1.704(5) . ?
Mo9 Ti1 3.0901(15) . ?
Mo9 K3 3.836(3) 2 ?
Mo9 O17 1.758(5) . ?
Mo9 O21 1.977(5) . ?
Mo9 O29 2.150(5) . ?
Mo9 O32 2.435(4) . ?
Mo9 O33 1.825(5) . ?
Mo9 O35 1.709(5) . ?
Ti1 Ti1 3.081(3) 2_565 ?
Ti1 O20 2.065(5) . ?
Ti1 O21 1.923(5) . ?
Ti1 O29 1.923(5) . ?
Ti1 O30 1.925(4) . ?
Ti1 O45 1.940(5) 2_565 ?
Ti1 O45 1.936(5) . ?
K1 Mo4 3.807(3) 2_666 ?
K1 Mo5 3.742(3) 2_666 ?
K1 P1 3.846(3) 2_666 ?
K1 O4 2.757(7) . ?
K1 O9 2.807(7) . ?
K1 O15 3.373(6) 2_666 ?
K1 O16 3.252(6) 2_666 ?
K1 O18 2.839(7) 2_666 ?
K1 O22 2.822(7) 2_666 ?
K1 O24 3.285(6) 2_666 ?
K1 O39 2.754(9) 2_666 ?
K1 O39 2.654(10) . ?
K2 Mo3 3.854(2) 2 ?
K2 Mo8 3.687(2) 2 ?
K2 K3 4.836(4) 2 ?
K2 O12 2.877(5) 2 ?
K2 O14 2.821(7) 2 ?
K2 O27 2.805(6) 2_565 ?
K2 O34 3.035(6) 2 ?
K2 O35 2.686(6) . ?
K2 O36 3.260(9) . ?
K2 O42 2.956(11) 2_565 ?
K3 Mo4 4.004(3) 2 ?
K3 Mo9 3.836(3) 2 ?
K3 K2 4.836(4) 2 ?
K3 O10 3.123(7) 2_655 ?
K3 O17 3.022(6) 2 ?
K3 O19 2.970(7) 2 ?
K3 O34 2.766(6) . ?
K3 O35 3.188(6) 2 ?
K3 O36 3.313(10) . ?
K3 O37 2.672(10) . ?
P1 K1 3.846(3) 2_666 ?
P1 O6 1.531(5) . ?
P1 O15 1.527(5) . ?
P1 O24 1.531(5) . ?
P1 O32 1.574(4) . ?
O10 K3 3.123(7) 2_655 ?
O12 K2 2.877(5) 2 ?
O14 K2 2.821(7) 2 ?
O15 K1 3.373(6) 2_666 ?
O16 K1 3.252(6) 2_666 ?
O17 K3 3.022(6) 2 ?
O18 K1 2.839(7) 2_666 ?
O19 K3 2.970(7) 2 ?
O22 K1 2.822(7) 2_666 ?
O24 K1 3.285(6) 2_666 ?
O27 K2 2.805(6) 2_565 ?
O34 K2 3.035(6) 2 ?
O35 K3 3.188(6) 2 ?
O39 K1 2.754(9) 2_666 ?
O45 Ti1 1.940(5) 2_565 ?
O42 K2 2.956(11) 2_565 ?

loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle_publ_flag
O1 Mo1 O2 82.3(2) . . ?
O1 Mo1 O3 153.7(2) . . ?
O1 Mo1 O6 72.8(2) . . ?
O2 Mo1 O6 79.58(17) . . ?
O3 Mo1 O2 79.5(2) . . ?
O3 Mo1 O6 85.4(2) . . ?
O4 Mo1 O1 97.9(3) . . ?
O4 Mo1 O2 167.3(2) . . ?
O4 Mo1 O3 95.8(3) . . ?
O4 Mo1 O6 88.3(2) . . ?
O5 Mo1 O1 98.4(3) . . ?
O5 Mo1 O2 89.3(2) . . ?
O5 Mo1 O3 100.2(3) . . ?
O5 Mo1 O4 103.2(3) . . ?
O5 Mo1 O6 166.5(2) . . ?
O1 Mo2 O6 72.5(2) . . ?
O1 Mo2 O8 82.0(2) . . ?
O7 Mo2 O1 152.6(2) . . ?
O7 Mo2 O6 85.1(2) . . ?
O7 Mo2 O8 78.4(2) . . ?
O8 Mo2 O6 79.17(18) . . ?
O9 Mo2 O1 97.1(3) . . ?
O9 Mo2 O6 87.7(3) . . ?
O9 Mo2 O7 97.4(3) . . ?
O9 Mo2 O8 166.5(3) . . ?
O10 Mo2 O1 96.9(3) . . ?
O10 Mo2 O6 165.9(3) . . ?
O10 Mo2 O7 102.1(3) . . ?
O10 Mo2 O8 90.2(3) . . ?
O10 Mo2 O9 103.3(3) . . ?
O7 Mo3 K2 90.75(18) . 2 ?
O7 Mo3 O11 152.2(2) . . ?
O7 Mo3 O12 78.7(2) . . ?
O7 Mo3 O15 83.7(2) . . ?
O11 Mo3 K2 91.97(18) . 2 ?
O11 Mo3 O12 82.7(2) . . ?
O11 Mo3 O15 72.7(2) . . ?
O12 Mo3 K2 47.65(13) . 2 ?
O12 Mo3 O15 79.98(18) . . ?
O13 Mo3 K2 145.2(2) . 2 ?
O13 Mo3 O7 96.2(3) . . ?
O13 Mo3 O11 97.2(3) . . ?
O13 Mo3 O12 166.9(3) . . ?
O13 Mo3 O14 103.4(3) . . ?
O13 Mo3 O15 87.5(3) . . ?
O14 Mo3 K2 41.9(2) . 2 ?
O14 Mo3 O7 102.6(3) . . ?
O14 Mo3 O11 97.9(3) . . ?
O14 Mo3 O12 89.6(2) . . ?
O14 Mo3 O15 166.6(2) . . ?
O15 Mo3 K2 127.24(12) . 2 ?
K1 Mo4 K3 152.21(8) 2_666 2 ?
O11 Mo4 K1 118.81(17) . 2_666 ?
O11 Mo4 K3 87.88(17) . 2 ?
O11 Mo4 O15 73.4(2) . . ?
O11 Mo4 O16 152.2(2) . . ?
O11 Mo4 O17 80.9(2) . . ?
O15 Mo4 K1 61.01(13) . 2_666 ?
O15 Mo4 K3 126.91(13) . 2 ?
O16 Mo4 K1 58.67(18) . 2_666 ?
O16 Mo4 K3 94.27(18) . 2 ?
O16 Mo4 O15 83.3(2) . . ?
O16 Mo4 O17 80.1(2) . . ?
O17 Mo4 K1 123.96(13) . 2_666 ?
O17 Mo4 K3 48.24(13) . 2 ?
O17 Mo4 O15 79.46(17) . . ?
O18 Mo4 K1 44.1(2) . 2_666 ?
O18 Mo4 K3 145.9(2) . 2 ?
O18 Mo4 O11 98.6(3) . . ?
O18 Mo4 O15 86.8(2) . . ?
O18 Mo4 O16 95.0(3) . . ?
O18 Mo4 O17 165.8(2) . . ?
O19 Mo4 K1 131.0(2) . 2_666 ?
O19 Mo4 K3 42.2(2) . 2 ?
O19 Mo4 O11 98.6(3) . . ?
O19 Mo4 O15 167.9(3) . . ?
O19 Mo4 O16 101.5(3) . . ?
O19 Mo4 O17 90.3(2) . . ?
O19 Mo4 O18 103.7(3) . . ?
Ti1 Mo5 K1 135.29(6) . 2_666 ?
O16 Mo5 Ti1 118.32(17) . . ?
O16 Mo5 K1 60.36(18) . 2_666 ?
O16 Mo5 O20 150.9(2) . . ?
O16 Mo5 O21 84.3(2) . . ?
O16 Mo5 O24 84.1(2) . . ?
O20 Mo5 Ti1 38.73(14) . . ?
O20 Mo5 K1 119.02(15) . 2_666 ?
O20 Mo5 O21 73.79(19) . . ?
O20 Mo5 O24 73.22(18) . . ?
O21 Mo5 Ti1 35.23(12) . . ?
O21 Mo5 K1 126.35(14) . 2_666 ?
O21 Mo5 O24 78.65(17) . . ?
O22 Mo5 Ti1 133.9(2) . . ?
O22 Mo5 K1 45.6(2) . 2_666 ?
O22 Mo5 O16 99.5(3) . . ?
O22 Mo5 O20 96.0(2) . . ?
O22 Mo5 O21 161.9(2) . . ?
O22 Mo5 O24 84.1(2) . . ?
O23 Mo5 Ti1 93.3(2) . . ?
O23 Mo5 K1 131.4(2) . 2_666 ?
O23 Mo5 O16 103.1(3) . . ?
O23 Mo5 O20 96.9(3) . . ?
O23 Mo5 O21 92.9(2) . . ?
O23 Mo5 O22 103.4(3) . . ?
O23 Mo5 O24 168.4(2) . . ?
O24 Mo5 Ti1 75.22(12) . . ?
O24 Mo5 K1 60.07(13) . 2_666 ?
O3 Mo6 Ti1 118.55(16) . . ?
O3 Mo6 O20 150.7(2) . . ?
O3 Mo6 O24 84.4(2) . . ?
O3 Mo6 O30 84.3(2) . . ?
O20 Mo6 Ti1 38.91(14) . . ?
O20 Mo6 O24 72.23(18) . . ?
O20 Mo6 O30 74.08(19) . . ?
O24 Mo6 Ti1 74.83(11) . . ?
O26 Mo6 Ti1 134.1(2) . . ?
O26 Mo6 O3 99.4(3) . . ?
O26 Mo6 O20 95.9(3) . . ?
O26 Mo6 O24 85.1(2) . . ?
O26 Mo6 O30 162.5(2) . . ?
O27 Mo6 Ti1 92.9(2) . . ?
O27 Mo6 O3 103.2(3) . . ?
O27 Mo6 O20 97.4(2) . . ?
O27 Mo6 O24 167.7(2) . . ?
O27 Mo6 O26 103.0(3) . . ?
O27 Mo6 O30 92.7(3) . . ?
O30 Mo6 Ti1 35.42(12) . . ?
O30 Mo6 O24 78.24(17) . . ?
O2 Mo7 Ti1 124.52(17) . . ?
O2 Mo7 O28 100.5(2) . . ?
O2 Mo7 O29 155.3(2) . . ?
O2 Mo7 O30 88.6(2) . . ?
O2 Mo7 O32 87.77(19) . . ?
O28 Mo7 Ti1 124.18(16) . . ?
O28 Mo7 O29 87.9(2) . . ?
O28 Mo7 O30 153.3(2) . . ?
O28 Mo7 O32 74.64(19) . . ?
O29 Mo7 Ti1 37.84(14) . . ?
O29 Mo7 O32 71.89(16) . . ?
O30 Mo7 Ti1 36.98(13) . . ?
O30 Mo7 O29 74.60(18) . . ?
O30 Mo7 O32 80.78(17) . . ?
O31 Mo7 Ti1 97.1(2) . . ?
O31 Mo7 O2 104.6(2) . . ?
O31 Mo7 O28 101.9(3) . . ?
O31 Mo7 O29 96.2(2) . . ?
O31 Mo7 O30 99.9(2) . . ?
O31 Mo7 O32 167.6(2) . . ?
O32 Mo7 Ti1 75.92(11) . . ?
O8 Mo8 K2 104.49(18) . 2 ?
O8 Mo8 O28 89.2(2) . . ?
O8 Mo8 O32 85.4(2) . . ?
O8 Mo8 O33 155.8(2) . . ?
O12 Mo8 K2 49.61(17) . 2 ?
O12 Mo8 O8 97.8(2) . . ?
O12 Mo8 O28 155.6(2) . . ?
O12 Mo8 O32 85.1(2) . . ?
O12 Mo8 O33 87.8(2) . . ?
O28 Mo8 K2 150.26(14) . 2 ?
O28 Mo8 O32 72.11(18) . . ?
O28 Mo8 O33 76.94(19) . . ?
O32 Mo8 K2 134.23(12) . 2 ?
O33 Mo8 K2 97.06(14) . 2 ?
O33 Mo8 O32 71.61(17) . . ?
O34 Mo8 K2 54.5(2) . 2 ?
O34 Mo8 O8 105.0(3) . . ?
O34 Mo8 O12 104.0(3) . . ?
O34 Mo8 O28 96.7(2) . . ?
O34 Mo8 O32 164.9(2) . . ?
O34 Mo8 O33 96.4(2) . . ?
Ti1 Mo9 K3 130.73(6) . 2 ?
O17 Mo9 Ti1 124.93(16) . . ?
O17 Mo9 K3 49.98(16) . 2 ?
O17 Mo9 O21 89.1(2) . . ?
O17 Mo9 O29 155.0(2) . . ?
O17 Mo9 O32 86.97(19) . . ?
O17 Mo9 O33 99.3(2) . . ?
O21 Mo9 Ti1 37.00(13) . . ?
O21 Mo9 K3 102.39(14) . 2 ?
O21 Mo9 O29 74.69(19) . . ?
O21 Mo9 O32 80.57(17) . . ?
O29 Mo9 Ti1 37.97(14) . . ?
O29 Mo9 K3 151.46(13) . 2 ?
O29 Mo9 O32 71.86(16) . . ?
O32 Mo9 Ti1 76.13(11) . . ?
O32 Mo9 K3 136.38(12) . 2 ?
O33 Mo9 Ti1 124.56(15) . . ?
O33 Mo9 K3 102.39(15) . 2 ?
O33 Mo9 O21 153.30(19) . . ?
O33 Mo9 O29 88.1(2) . . ?
O33 Mo9 O32 74.68(18) . . ?
O35 Mo9 Ti1 97.08(19) . . ?
O35 Mo9 K3 55.24(19) . 2 ?
O35 Mo9 O17 104.8(2) . . ?
O35 Mo9 O21 99.9(2) . . ?
O35 Mo9 O29 96.8(2) . . ?
O35 Mo9 O32 168.2(2) . . ?
O35 Mo9 O33 102.2(2) . . ?
Mo6 Ti1 Mo5 65.12(3) . . ?
Mo7 Ti1 Mo5 113.39(4) . . ?
Mo7 Ti1 Mo6 76.58(3) . . ?
Mo9 Ti1 Mo5 76.51(3) . . ?
Mo9 Ti1 Mo6 114.08(4) . . ?
Mo9 Ti1 Mo7 72.33(3) . . ?
Ti1 Ti1 Mo5 122.01(7) 2_565 . ?
Ti1 Ti1 Mo6 120.52(7) 2_565 . ?
Ti1 Ti1 Mo7 124.21(7) 2_565 . ?
Ti1 Ti1 Mo9 125.16(6) 2_565 . ?
O20 Ti1 Mo5 38.21(14) . . ?
O20 Ti1 Mo6 38.36(14) . . ?
O20 Ti1 Mo7 112.67(15) . . ?
O20 Ti1 Mo9 112.70(15) . . ?
O20 Ti1 Ti1 106.64(16) . 2_565 ?
O21 Ti1 Mo5 39.48(14) . . ?
O21 Ti1 Mo6 95.40(14) . . ?
O21 Ti1 Mo7 99.06(15) . . ?
O21 Ti1 Mo9 38.21(14) . . ?
O21 Ti1 Ti1 127.47(15) . 2_565 ?
O21 Ti1 O20 77.5(2) . . ?
O21 Ti1 O30 106.4(2) . . ?
O21 Ti1 O45 90.1(2) . . ?
O21 Ti1 O45 164.6(2) . 2_565 ?
O29 Ti1 Mo5 117.09(15) . . ?
O29 Ti1 Mo6 116.98(14) . . ?
O29 Ti1 Mo7 42.94(14) . . ?
O29 Ti1 Mo9 43.48(14) . . ?
O29 Ti1 Ti1 109.35(15) . 2_565 ?
O29 Ti1 O20 144.0(2) . . ?
O29 Ti1 O21 81.4(2) . . ?
O29 Ti1 O30 80.9(2) . . ?
O29 Ti1 O45 104.7(3) . 2_565 ?
O29 Ti1 O45 105.8(2) . . ?
O30 Ti1 Mo5 94.94(14) . . ?
O30 Ti1 Mo6 39.51(14) . . ?
O30 Ti1 Mo7 38.20(14) . . ?
O30 Ti1 Mo9 99.27(15) . . ?
O30 Ti1 Ti1 125.86(16) . 2_565 ?
O30 Ti1 O20 77.6(2) . . ?
O30 Ti1 O45 88.6(2) . 2_565 ?
O30 Ti1 O45 163.1(2) . . ?
O45 Ti1 Mo5 95.58(19) . . ?
O45 Ti1 Mo5 138.1(2) 2_565 . ?
O45 Ti1 Mo6 137.2(2) . . ?
O45 Ti1 Mo6 94.28(18) 2_565 . ?
O45 Ti1 Mo7 144.3(2) . . ?
O45 Ti1 Mo7 94.77(18) 2_565 . ?
O45 Ti1 Mo9 144.0(2) 2_565 . ?
O45 Ti1 Mo9 96.04(18) . . ?
O45 Ti1 Ti1 37.42(16) . 2_565 ?
O45 Ti1 Ti1 37.31(15) 2_565 2_565 ?
O45 Ti1 O20 103.3(3) 2_565 . ?
O45 Ti1 O20 103.0(3) . . ?
O45 Ti1 O45 74.7(2) . 2_565 ?
Mo4 K1 P1 55.66(5) 2_666 2_666 ?
Mo5 K1 Mo4 59.11(5) 2_666 2_666 ?
Mo5 K1 P1 55.85(5) 2_666 2_666 ?
O4 K1 Mo4 100.03(15) . 2_666 ?
O4 K1 Mo5 138.73(17) . 2_666 ?
O4 K1 P1 144.01(18) . 2_666 ?
O4 K1 O9 68.0(2) . . ?
O4 K1 O15 121.67(19) . 2_666 ?
O4 K1 O16 118.01(19) . 2_666 ?
O4 K1 O18 75.66(18) . 2_666 ?
O4 K1 O22 132.4(2) . 2_666 ?
O4 K1 O24 165.18(19) . 2_666 ?
O9 K1 Mo4 141.16(17) . 2_666 ?
O9 K1 Mo5 104.77(15) . 2_666 ?
O9 K1 P1 147.83(17) . 2_666 ?
O9 K1 O15 169.53(19) . 2_666 ?
O9 K1 O16 121.79(19) . 2_666 ?
O9 K1 O18 130.7(2) . 2_666 ?
O9 K1 O22 80.07(19) . 2_666 ?
O9 K1 O24 125.87(19) . 2_666 ?
O15 K1 Mo4 38.18(9) 2_666 2_666 ?
O15 K1 Mo5 65.50(10) 2_666 2_666 ?
O15 K1 P1 23.25(9) 2_666 2_666 ?
O16 K1 Mo4 30.35(10) 2_666 2_666 ?
O16 K1 Mo5 29.80(10) 2_666 2_666 ?
O16 K1 P1 55.55(10) 2_666 2_666 ?
O16 K1 O15 51.56(14) 2_666 2_666 ?
O16 K1 O24 52.16(13) 2_666 2_666 ?
O18 K1 Mo4 24.81(11) 2_666 2_666 ?
O18 K1 Mo5 81.57(14) 2_666 2_666 ?
O18 K1 P1 75.74(13) 2_666 2_666 ?
O18 K1 O15 53.92(15) 2_666 2_666 ?
O18 K1 O16 51.77(16) 2_666 2_666 ?
O18 K1 O24 89.96(15) 2_666 2_666 ?
O22 K1 Mo4 83.10(14) 2_666 2_666 ?
O22 K1 Mo5 25.64(12) 2_666 2_666 ?
O22 K1 P1 75.49(13) 2_666 2_666 ?
O22 K1 O15 89.76(16) 2_666 2_666 ?
O22 K1 O16 52.77(16) 2_666 2_666 ?
O22 K1 O18 102.9(2) 2_666 2_666 ?
O22 K1 O24 53.80(15) 2_666 2_666 ?
O24 K1 Mo4 66.02(9) 2_666 2_666 ?
O24 K1 Mo5 39.12(9) 2_666 2_666 ?
O24 K1 P1 23.13(9) 2_666 2_666 ?
O24 K1 O15 44.12(13) 2_666 2_666 ?
O39 K1 Mo4 130.7(2) 2_666 2_666 ?
O39 K1 Mo4 89.4(2) . 2_666 ?
O39 K1 Mo5 131.5(2) . 2_666 ?
O39 K1 Mo5 94.9(2) 2_666 2_666 ?
O39 K1 P1 75.0(2) 2_666 2_666 ?
O39 K1 P1 76.2(2) . 2_666 ?
O39 K1 O4 122.6(2) 2_666 . ?
O39 K1 O4 77.7(3) . . ?
O39 K1 O9 121.3(3) . . ?
O39 K1 O9 82.3(2) 2_666 . ?
O39 K1 O15 67.3(2) . 2_666 ?
O39 K1 O15 94.3(2) 2_666 2_666 ?
O39 K1 O16 116.1(2) . 2_666 ?
O39 K1 O16 119.4(2) 2_666 2_666 ?
O39 K1 O18 79.8(3) . 2_666 ?
O39 K1 O18 146.6(3) 2_666 2_666 ?
O39 K1 O22 84.9(3) 2_666 2_666 ?
O39 K1 O22 149.8(3) . 2_666 ?
O39 K1 O24 68.3(2) 2_666 2_666 ?
O39 K1 O24 96.5(2) . 2_666 ?
O39 K1 O39 78.0(3) . 2_666 ?
Mo3 K2 K3 118.17(7) 2 2 ?
Mo8 K2 Mo3 59.92(4) 2 2 ?
Mo8 K2 K3 58.29(6) 2 2 ?
O12 K2 Mo3 34.30(10) 2 2 ?
O12 K2 Mo8 27.89(10) 2 2 ?
O12 K2 K3 85.20(12) 2 2 ?
O12 K2 O34 55.01(14) 2 2 ?
O12 K2 O36 59.56(16) 2 . ?
O12 K2 O42 118.3(2) 2 2_565 ?
O14 K2 Mo3 24.00(12) 2 2 ?
O14 K2 Mo8 83.36(13) 2 2 ?
O14 K2 K3 140.99(14) 2 2 ?
O14 K2 O12 58.30(16) 2 2 ?
O14 K2 O34 109.20(17) 2 2 ?
O14 K2 O36 81.47(18) 2 . ?
O14 K2 O42 92.8(2) 2 2_565 ?
O27 K2 Mo3 128.54(15) 2_565 2 ?
O27 K2 Mo8 148.44(16) 2_565 2 ?
O27 K2 K3 103.95(16) 2_565 2 ?
O27 K2 O12 157.62(18) 2_565 2 ?
O27 K2 O14 106.1(2) 2_565 2 ?
O27 K2 O34 127.54(19) 2_565 2 ?
O27 K2 O36 138.64(19) 2_565 . ?
O27 K2 O42 75.6(2) 2_565 2_565 ?
O34 K2 Mo3 86.57(11) 2 2 ?
O34 K2 Mo8 27.21(10) 2 2 ?
O34 K2 K3 31.81(11) 2 2 ?
O34 K2 O36 84.54(17) 2 . ?
O35 K2 Mo3 140.18(15) . 2 ?
O35 K2 Mo8 87.49(13) . 2 ?
O35 K2 K3 38.11(12) . 2 ?
O35 K2 O12 107.71(17) . 2 ?
O35 K2 O14 159.4(2) . 2 ?
O35 K2 O27 91.26(19) . 2_565 ?
O35 K2 O34 66.08(16) . 2 ?
O35 K2 O36 78.14(17) . . ?
O35 K2 O42 80.66(19) . 2_565 ?
O36 K2 Mo3 70.61(13) . 2 ?
O36 K2 Mo8 71.74(13) . 2 ?
O36 K2 K3 92.03(14) . 2 ?
O42 K2 Mo3 105.51(17) 2_565 2 ?
O42 K2 Mo8 134.92(19) 2_565 2 ?
O42 K2 K3 118.53(16) 2_565 2 ?
O42 K2 O34 138.0(2) 2_565 2 ?
O42 K2 O36 63.3(2) 2_565 . ?
Mo4 K3 K2 114.30(8) 2 2 ?
Mo9 K3 Mo4 58.64(4) 2 2 ?
Mo9 K3 K2 55.74(5) 2 2 ?
O10 K3 Mo4 95.38(13) 2_655 2 ?
O10 K3 Mo9 142.05(16) 2_655 2 ?
O10 K3 K2 136.49(15) 2_655 2 ?
O10 K3 O35 141.9(2) 2_655 2 ?
O10 K3 O36 135.4(2) 2_655 . ?
O17 K3 Mo4 33.06(10) 2 2 ?
O17 K3 Mo9 26.45(10) 2 2 ?
O17 K3 K2 81.96(12) 2 2 ?
O17 K3 O10 126.13(18) 2 2_655 ?
O17 K3 O35 52.45(14) 2 2 ?
O17 K3 O36 58.70(16) 2 . ?
O19 K3 Mo4 22.70(11) 2 2 ?
O19 K3 Mo9 80.72(12) 2 2 ?
O19 K3 K2 135.61(14) 2 2 ?
O19 K3 O10 73.45(17) 2 2_655 ?
O19 K3 O17 55.71(15) 2 2 ?
O19 K3 O35 104.27(16) 2 2 ?
O19 K3 O36 82.71(19) 2 . ?
O34 K3 Mo4 134.11(15) . 2 ?
O34 K3 Mo9 81.21(14) . 2 ?
O34 K3 K2 35.33(13) . 2 ?
O34 K3 O10 130.42(19) . 2_655 ?
O34 K3 O17 102.90(17) . 2 ?
O34 K3 O19 154.9(2) . 2 ?
O34 K3 O35 63.04(16) . 2 ?
O34 K3 O36 73.96(18) . . ?
O35 K3 Mo4 83.45(11) 2 2 ?
O35 K3 Mo9 26.14(9) 2 2 ?
O35 K3 K2 31.34(10) 2 2 ?
O35 K3 O36 80.00(17) 2 . ?
O36 K3 Mo4 69.86(13) . 2 ?
O36 K3 Mo9 65.50(13) . 2 ?
O36 K3 K2 86.30(14) . 2 ?
O37 K3 Mo4 67.3(2) . 2 ?
O37 K3 Mo9 69.92(18) . 2 ?
O37 K3 K2 87.8(2) . 2 ?
O37 K3 O10 74.7(2) . 2_655 ?
O37 K3 O17 70.8(2) . 2 ?
O37 K3 O19 67.6(3) . 2 ?
O37 K3 O34 121.4(3) . . ?
O37 K3 O35 69.7(2) . 2 ?
O37 K3 O36 129.5(2) . . ?
O6 P1 K1 100.1(2) . 2_666 ?
O6 P1 O24 110.4(3) . . ?
O6 P1 O32 108.3(3) . . ?
O15 P1 K1 60.7(2) . 2_666 ?
O15 P1 O6 109.8(3) . . ?
O15 P1 O24 109.8(3) . . ?
O15 P1 O32 108.4(3) . . ?
O24 P1 K1 57.40(19) . 2_666 ?
O24 P1 O32 110.0(3) . . ?
O32 P1 K1 151.56(19) . 2_666 ?
Mo1 O1 Mo2 121.1(3) . . ?
Mo7 O2 Mo1 150.2(3) . . ?
Mo6 O3 Mo1 158.6(3) . . ?
Mo1 O4 K1 137.5(3) . . ?
Mo2 O6 Mo1 90.03(16) . . ?
P1 O6 Mo1 130.7(3) . . ?
P1 O6 Mo2 129.8(3) . . ?
Mo2 O7 Mo3 161.2(3) . . ?
Mo8 O8 Mo2 143.1(3) . . ?
Mo2 O9 K1 137.3(3) . . ?
Mo2 O10 K3 135.9(3) . 2_655 ?
Mo4 O11 Mo3 121.6(3) . . ?
Mo3 O12 K2 98.04(18) . 2 ?
Mo8 O12 Mo3 144.0(3) . . ?
Mo8 O12 K2 102.5(2) . 2 ?
Mo3 O14 K2 114.1(3) . 2 ?
Mo3 O15 K1 124.70(18) . 2_666 ?
Mo4 O15 Mo3 88.59(17) . . ?
Mo4 O15 K1 80.81(15) . 2_666 ?
P1 O15 Mo3 129.2(3) . . ?
P1 O15 Mo4 130.8(3) . . ?
P1 O15 K1 96.0(2) . 2_666 ?
Mo4 O16 K1 91.0(2) . 2_666 ?
Mo5 O16 Mo4 159.6(3) . . ?
Mo5 O16 K1 89.8(2) . 2_666 ?
Mo4 O17 K3 98.69(17) . 2 ?
Mo9 O17 Mo4 150.9(3) . . ?
Mo9 O17 K3 103.6(2) . 2 ?
Mo4 O18 K1 111.1(3) . 2_666 ?
Mo4 O19 K3 115.1(3) . 2 ?
Mo5 O20 Ti1 103.1(2) . . ?
Mo6 O20 Mo5 115.7(2) . . ?
Mo6 O20 Ti1 102.7(2) . . ?
Mo9 O21 Mo5 144.9(2) . . ?
Ti1 O21 Mo5 105.3(2) . . ?
Ti1 O21 Mo9 104.8(2) . . ?
Mo5 O22 K1 108.8(3) . 2_666 ?
Mo5 O24 Mo6 91.42(17) . . ?
Mo5 O24 K1 80.81(15) . 2_666 ?
Mo6 O24 K1 121.14(18) . 2_666 ?
P1 O24 Mo5 128.6(3) . . ?
P1 O24 Mo6 128.0(3) . . ?
P1 O24 K1 99.5(2) . 2_666 ?
Mo6 O27 K2 138.6(3) . 2_565 ?
Mo7 O28 Mo8 121.9(3) . . ?
Mo7 O29 Mo9 116.8(2) . . ?
Ti1 O29 Mo7 99.2(2) . . ?
Ti1 O29 Mo9 98.6(2) . . ?
Mo7 O30 Mo6 145.2(2) . . ?
Ti1 O30 Mo6 105.1(2) . . ?
Ti1 O30 Mo7 104.8(2) . . ?
Mo8 O32 Mo7 89.57(15) . . ?
Mo8 O32 Mo9 90.56(15) . . ?
Mo9 O32 Mo7 96.77(15) . . ?
P1 O32 Mo7 123.1(2) . . ?
P1 O32 Mo8 124.0(3) . . ?
P1 O32 Mo9 123.6(2) . . ?
Mo9 O33 Mo8 121.8(2) . . ?
Mo8 O34 K2 98.2(2) . 2 ?
Mo8 O34 K3 144.6(3) . . ?
K3 O34 K2 112.86(19) . 2 ?
Mo9 O35 K2 140.4(3) . . ?
Mo9 O35 K3 98.6(2) . 2 ?
K2 O35 K3 110.54(17) . 2 ?
K2 O36 K3 170.8(2) . . ?
K1 O39 K1 102.1(3) . 2_666 ?
Ti1 O45 Ti1 105.3(2) . 2_565 ?


_olex2_submission_special_instructions 'No special instructions were received'
